The advent of clad coinage in 1965 expanded the number and variety
of planchet errors available to the collector.
The process of fabricating and then bonding two coils of clad
strip to a middle coil of core strip invites numerous mishaps as does
the subsequent rolling of the composite strip to coin thickness.
One of the rarest bonding errors is the “struck core,” wherein
both clad layers fall away after the blank is punched out. While it’s
common for one clad layer to fall off after blanking, I have only seen
or heard of a handful of cases where both layers have been lost. They
include two Roosevelt dimes struck on copper cores (both shown here),
two to three Washington quarter dollars struck on copper cores, and a
1965 Kennedy half dollar struck on a 79 percent copper and 21 percent
silver core. All are naturally quite thin and significantly
underweight, and most show weakness in the strike.
Most struck cores are thought to be the result of improper
cleaning. Both sides of the core strip and the internal surface of
each clad strip must be meticulously cleaned prior to bonding. The
surfaces are scoured clean by rotating descaling brushes that often
leave fine striations on the surface.
Our first illustrated coin is a 1969-D Roosevelt dime struck on a
copper core. Since each copper-nickel clad layer weighs approximately
0.4 gram, the expected weight of the core alone would be 1.47 grams.
The reported weight of this dime is 1.4 grams, which is close enough
to clinch the diagnosis.
The weakly-struck areas on either face show no fine striations,
which may mean that this portion of the strip wasn’t cleaned at all.
This conclusion is not certain however, as the presence and
distinctness of striations is somewhat variable in the more commonly
seen counterpart to this error, the isolated struck clad layer.
Our second piece is a 1981-P Roosevelt dime struck on very
different-looking copper core. A small island of gray metal appears on
the right side of the obverse face and a few flecks of gray metal on
the reverse face. I have my doubts that the gray metal is remnant
cladding because the southern tip of the obverse patch actually dives
beneath an adjacent flap of copper.
Cladding should always occupy a superficial position relative to
the core. I believe that either copper atoms migrated so as to partly
envelop this island of cladding, or this dark gray patch represents an
area of core material enriched by migrating nickel atoms.
At 1.3 grams, the coin is a bit lighter than expected. The reason
is immediately apparent on close inspection. Before and after the coin
was struck, moderately thick layers of copper spalled off the obverse
face in several places, exposing interior metal with a fine matte
texture. Even the intact portions of the obverse surface show cracking
The features described above are consistent with an improper
annealing error. Such errors occur when copper-nickel clad or solid
copper-nickel planchets are exposed to excessive heat or when oxygen
floods the annealing oven. Within the alloy, copper and nickel
fractions tend to segregate out (copper usually to the surface). Areas
of copper-nickel often darken to a gray or black color. Planchets
become brittle, the surface often cracking and flaking. Metal exposed
by missing flakes has the aforementioned fine matte texture.
In the case of this 1981-P dime, it’s likely that the intense heat
weakened the bond between the clad layers and the core, causing
separation after blanking. The heat also rendered the core brittle and
friable. Given this scenario, one would expect to find some
single-sided missing clad errors with the characteristics of an
improper annealing error, but I have yet to encounter one.
Coin World’s Collectors’ Clearinghouse department does
not accept coins or other items for examination without prior
permission from News Editor William T. Gibbs. Materials sent to
Clearinghouse without prior permission will be returned unexamined.
Please address all Clearinghouse inquiries to firstname.lastname@example.org or to
800-673-8311, Ext. 172.